w w w . s t a i n l e s s - s t e e l - w o r l d . n e t S t a i n l e s s S t e e l W o r l d O c t o b e r 2 0 1 3 1 CORROSION Corrosion taking place under insulating materials Introduction The corrosion that takes place under insulation material is a major problem. It has been a primary problem in the oil & gas, chemical, food processing, and other industries for many years and has cost many millions of dollars in inspection and repair of process pipes and pipelines. The American Petroleum Institute code, API 570 Inspection, Repair Alteration and Re-rating of In-service Piping Systems, (June 1993), identifies Corrosion Under Insulation (CUI) as a special concern. In 2003, the European Corrosion Federation reported that most leaks in the refining and chemical industries were due to CUI, rather than process leaks. When insulation material becomes wet (because of poor installation practices, subsequent abuse or failure to specify good vapor barriers and waterproofing materials), it creates the potential for corrosive failure of the piping. Whether pipes are above ground or buried, proper design and installation techniques can control corrosion. CUI is one of the predominant mechanical integrity issues affecting the ethylene industry. Occurrence can be erratic and sometimes undetectable based on visual examination. In addition to these recognized problem areas, it is also important to look for areas that are susceptible to CUI due to swing conditions or non-flow areas, even though the design and observed operating condition of the line fall outside this range. It results from the collection of water in the vapor space (or annulus space) between the insulation and the metal surface. Sources of water may include rain, water leaks, condensation, cooling water tower drift, deluge systems, and steam tracing leaks. CUI causes wall loss in the form of localized corrosion. Plants located in areas with high annual rainfall or warm, marine locations are more prone to CUI than plants located in cooler, drier, mid-continent locations. Units which are located near cooling towers and steam vents are highly susceptible to CUI, as are units whose operating temperature cycle through the dew point on a regular basis. The external inspection of insulated systems should include a review of the integrity of the insulation system for conditions that could lead to CUI and for signs of ongoing CUI, i.e. rust stains or bulging. Prevention of CUI can be carried out through proper coating and good insulation practices. Good installation and maintenance of insulation prevents ingress of large quantities of water. A coating system is frequently specified for component operating in the CUI temperature range, and where CUI has been a problem. A good coating system should last a minimum of fifteen years. Currently there are few reliable inspection and monitoring techniques and so new sensors for CUI inspection. Major factors which affect CUI It affects externally insulated piping and equipment and those that are in intermittent service or operate between 12C to 175C for carbon Fig.1. An insulated pipeline, which faced corrosion in a petrochemical plant. CUI takes place under insulating material in the oil & gas, chemical, and food processing industries, to name but a few industries affected, costs millions of dollars on a yearly basis. In this article, the major factors that lead to corrosion under insulation are examined and the major types of units and equipment that get affected are discussed. CUI appearance is also discussed. Further, an important section of the article looks at how corrosion under insulating materials can be prevented, as well as preventive inspection and monitoring practices, including the use of a probe array sensor inserted to detect its formation at thermally insulated pipeline field joints. By Dr. Arwind Kumar Dubey, Senior Integrity Engineer, Intertek, Dubai, United Arab Emirates
2 S t a i n l e s s S t e e l W o r l d O c t o b e r 2 0 1 3 w w w . s t a i n l e s s - s t e e l - w o r l d . n e t CORROSION and low alloy steels whereas 60C to 205C for austenitic stainless steels and duplex stainless steels. Corrosion rates increase with increasing metal temperature up to the point where the water evaporates quickly. For insulated components, corrosion becomes more severe at metal temperatures between the boiling point 100C and 121C, where water is less likely to vaporize and insulation stays wet longer. Design of insulation system, insulation type, temperature and environment are critical factors. Poor design and/or installations that allow water to become trapped will increase CUI. Insulating materials that hold moisture (wick) can be more of a problem. Cyclic thermal operation or intermittent service can increase corrosion. Equipment that operates below the water dew point tends to condense water on the metal surface thus providing a wet environment and increasing the risk of corrosion. Damage is aggravated by contaminants that may be leached out of the insulation, such as chlorides. Plants located in areas with high annual rainfall or warmer, marine locations are more prone to CUI than plants located in cooler, drier, mid-continent locations. Environments that provide airborne contaminants such as chlorides (marine environments, cooling tower drift) or SO2 (stack emissions) can accelerate corrosion. Units or equipment which get affected by CUI Insulated equipment and piping are susceptible to CUI under conditions noted above even on piping and equipment where the insulation system appears to be in good condition and no visual signs of corrosion are present. CUI can be found on equipment with damaged insulation, vapor barriers, weather proofing or mastic, or protrusions through the insulation or at insulation termination points such as flanges. Equipment designed with insulation support rings welded directly to the vessel wall (no standoff); particularly around ladder and platform clips, and lifting lugs, nozzles and stiffener rings. Piping or equipment with damaged/leaking steam tracing. Localized damage at paint and/or coating systems. Locations where moisture/water will naturally collect (gravity drainage) before evaporating (insulation support rings on vertical equipment) and improperly terminated fireproofing. Vibrating piping systems that have a tendency to inflict damage to insulation jacketing providing a path for water ingress. Deadlegs Steam tracer tubing penetrations. Caulking that has hardened, has separated, or is missing. Bulges or staining of the insulation or jacketing system or missing bands. Low points in piping systems that have a known breach in the insulation system, including low points in long unsupported piping runs. Carbon or low-alloy steel flanges, bolting, and other components under insulation in high-alloy piping systems. Locations where insulation plugs have been removed to permit piping thickness measurements on insulated piping and equipment should receive particular attention. CUI appearance Carbon and low alloy steels are subject to localized pitting corrosion and or localized loss in thickness. 300 Series SS are also subject to Stress Corrosion Cracking (SCC) if chlorides are present, while the duplex SS are less susceptible. 300 Series SS and duplex SS are subject to pitting and localized corrosion. For 300 Series SS, specifically in older calcium silicate insulation (known to contain chlorides), localized pitting and chloride stress corrosion cracking can occur. After insulation is removed from carbon and low alloy steels, CUI damage often appears as loose, flaky scale covering the corroded component. Damage may be highly localized. In some localized cases, the corrosion can appear to be carbuncle type pitting (usually found under a failed paint/coating system). Fig. 2A & 2B show the appearance of CUI after the removal of insulating material in a petrochemical plant. (A) (B)
w w w . s t a i n l e s s - s t e e l - w o r l d . n e t S t a i n l e s s S t e e l W o r l d O c t o b e r 2 0 1 3 3 CORROSION Control of CUI Majority of construction materials used in plants are susceptible to CUI degradation, mitigation is best achieved by using appropriate paints/coatings and maintaining the insulation/sealing/vapor barriers to prevent moisture ingress. Flame-sprayed aluminum coatings have been used on carbon steels. The coating corrodes preferentially by galvanic action, thereby protecting the base metal. High quality non-metallic coatings, properly applied to the surfaces to be insulated can provide long term protection. Thin aluminum foil wrapped on stainless steel piping and equipment has been used on stainless steels as an effective barrier under insulation. Careful selection of insulating materials is important. Closed-cell foam glass materials will hold less water against the vessel/pipe wall than mineral wool and potentially be less corrosive. Low chloride insulation should be used on 300 Series SS to minimize the potential for pitting and chloride SCC. It is not usually possible to modify operating conditions. However, consideration should be given to removing the insulation on equipment where heat conservation is not as important. CUI inspection and monitoring An inspection plan for corrosion under insulation should be a structured and systematic approach starting with prediction/analysis, then looking at the more invasive procedures. The inspection plan should consider operating temperature; type and age/condition of coating; and type and age/condition of insulation material. Additional prioritization can be added from a physical inspection of the equipment, looking for evidence of insulation, mastic and/or sealant damage, signs of water penetration and rust in gravity drain areas around the equipment. Although external insulation may appear to be in good condition, CUI damage may still be occurring. CUI inspection may require removal of some or all insulation. If external coverings are in good condition and there is no reason to suspect damage behind them, it may not be necessary to remove them for inspection of the vessel. Considerations for insulation removal include history of CUI for the vessel or comparable equipment, visual condition of the external covering and insulation, evidence of fluid leakage, e.g. stains, equipment in intermittent service, condition/age of the external coating. Common areas of concern in process units are high moisture areas such as those down-winds from cooling towers, near steam vents, deluge systems, acid vapors, or near supplemental cooling with water spray. Inserted probe array sensor for CUI monitoring The Inserted Probe Array Sensor acts as a corrosionfuse detector that will provide an indication of corrosion occurring atthe pipe surface, at known discrete locations. It was originally designedto be installed during the remediation and mitigation of corrosiondamage under thermally insulated pipeline field joints. There are twocommon types of pipeline insulation repair processes. The firstrequires the old cladding to be removed with the insulation left in place.Insulation tape is wrapped around the affected area and anew protective cladding is strapped in place. The second involvesremoving an entire section of insulation from a damaged area. Thepipe is repaired and cleaned, and new insulation is installed. Insulatingtape is then applied and a protective outer cladding isstrapped in place. References 1. API 571-Damage Mechanisms Affecting Fixed Equipment in the Refining Industry. 2. Risk-Based Inspection Technology, API Recommended Practice 581. Fig. 3. A corrosion fuse inserted probe array sensor for CUI monitoring. About the author Dr. Arwind Kumar Dubey holds a Ph.D. degree in Corrosion Chemistry from the University of Delhi, Delhi, India and an MBA degree from an Indian University. He is certified by NACE as a Senior Corrosion Technologist and Coating Inspector Professional. Dr. Dubey has ten years work experience in R&D, oil/gas, refinery and petrochemicals engineering. His expertise is related to chemical treatment, coatings, material selection, corrosion protection, RBI (Risk Based Inspection), Meridium. He has worked in India, Oman, Saudi Arabia, and the United Arab Emirates. He has published many corrosion related research papers in international journals and is, furthermore, a reviewer of a number of chemical engineering journals e.g. the Polish Journal of Chemical Technology, Corrosion, the Indian Journal of Chemical Technology. Dr. Dubey is an individual member of NACE and is a Professional Member of the Institute of Corrosion (MICorr).